Designation: C 471M – 01 METRIC
Standard Test Methods for
Chemical Analysis of Gypsum and Gypsum Products [Metric]1 This standard is issued under the ﬁxed designation C 471M; the number immediately following the designation indicates the year of original adoption or, in the case of revision, the year of last revision. A number in parentheses indicates the year of last reapproval. A superscript superscript epsilon (e) indicates an editorial change since the last revision or reapproval.
1. Scope Scope * 1.1 These These test test method methodss cover cover the chemic chemical al analys analysis is of gypsum and gypsum products, including gypsum ready-mixed plaster, gypsum wood-ﬁbered plaster and gypsum concrete. NOTE 1—Gypsum reference standard materials, prepared by Domtar, Inc are available through Brammer Standards Company, Inc.
1.2 The test methods methods appear in the following following order: Sections Alternative Procedure for Analysis for Calcium Sulfate by Ammonium Acetate Method Alternative Procedure for Analysis for Sodium Chloride by the Coulometric Method Complete Procedure Determination of Sand in Set Plaster Optional Optional Procedure Procedure for Analysis Analysis for Sodium Sodium by Flame Flame Photometry Photometry Optional Procedure for Analysis for Sodium by the Atomic Absorption Method Preparation of Sample Wood-F od-Fib iber er C on ontent tent in Wood ood-Fi -Fiber ber Gyps Gypsu um Plas Plaste terr
17-22 23-29 5-16 30-36 47-54 40-46 4 37-3 37-39 9
1.3 The text of this standard standard references references notes and footnotes footnotes that provide explanatory material. These notes and footnotes (excluding those in tables and ﬁgures) shall not be considered as requirements of the standard. 1.4 The values values stated stated in SI units units are to be regard regarded ed as the standard. standard d does does not purport purport to addre address ss all of the 1.5 This standar safe safety ty conc concer erns ns,, if any any, asso associ ciat ated ed with with its use. use. It is the the responsibility of the user of this standard to establish appro priate safety and health practices and determine the applicability of regulatory limitations prior to use. 2. Referenced Documents 2.1 ASTM Standards: C 11 11 Terminolo erminology gy Relating Relating to Gypsum Gypsum and Related Related Gypsum Building Materials and Systems 2
These test methods are under the jurisdiction of ASTM Committee C11 on Gypsum and Related Building Materials and Systems and are the direct responsibility of Subcommittee Subcommittee C11.01 C11.01 on Speciﬁcations Speciﬁcations and Test Methods for Gypsum Gypsum Products. Current edition approved Dec. 10, 2001. Published February 2002. Originally published published as C 471 – 61. Last previous previous edition C 471 – 96. 2 Annual Book of ASTM Standards Standards , Vol 04.01.
C 22/C 22/C 22M Speciﬁcat Speciﬁcation ion for Gypsum Gypsum2 C 28 Speciﬁcat Speciﬁcation ion for Gypsum Gypsum Plasters Plasters2 C 59 Speciﬁcat Speciﬁcation ion for Gypsum Gypsum Casting Casting and Molding Molding Plas2 ter C 61 Speciﬁcat Speciﬁcation ion for Gypsum Gypsum Keene’s Keene’s Cement2 C 317 Speciﬁcati Speciﬁcation on for Gypsum Gypsum Concrete2 C 842 Speciﬁ Speciﬁcat cation ion for Applic Applicati ation on of Interi Interior or Gypsum Gypsum 2 Plaster D 1193 1193 Speciﬁcation for Reagent Water Water 3 D 1428 Methods of Test Test for Sodium and Potassium in Water Water and Water-Formed Deposits by Flame Photometry 3 D 2013 Method Method of Preparing Preparing Coal Samples for Analysis Analysis 4 E 11 11 Speciﬁcat Speciﬁcation ion for Wire-C Wire-Cloth loth and Sieves Sieves for Testing esting 5 Purposes 3. Terminology 3.1 Deﬁnitions—Deﬁni —Deﬁniti tions ons shall shall be in accord accordanc ancee with with Terminology C 11. 3.2 Deﬁnitions of Terms Speciﬁc to This Standard: 3.2.1 sample as received , n—a representative portion of raw gypsum or gypsum product in the state received by the testing laboratory, including aggregates, impurities and water content. 3.2.2 dried sample, n —a sample devoid of free water. 3.2.3 riffle, n—a hand hand feed feed samp sample le divi divide derr devi device ce that that divide dividess the sample sample into into parts parts of approx approxima imatel tely y the same same weight. (D 2013) 4. Preparat Preparation ion of Sample General Procedur Procedures es—Detai 4.1 General —Details ls of sample sample prepar preparati ation on will vary according to the type of material being tested. Samplee As Receiv Received ed —Use 4.1.1 Sampl —Use a suff sufficient icient amount amount of sample such that, after sieving, not less than 50 g of sample will remain for testing. Weigh the entire sample immediately after opening the container in which the material was received. This will become the weight of the sample as received. 4.1.2 Drying—Dry the sample in accordance with Section 7. This will be the weight of the dried sample.
Annual Book of ASTM Standards Standards,, Vol 11.01. Annual Book of ASTM Standards Standards,, Vol 05.05. 5 Annual Book of ASTM Standards Standards,, Vol 14.02. 4
*A Summary of Changes section appears at the end of this standard.
C 471M 4.1.3 Crushing and Grinding—Crush and grind the sample by hand with a mortar and pestle or by mechanical crushing and grinding equipment to pass a 250-µm (No. 60) sieve. Take care, particularly with mechanical equipment, not to expose the sample to temperatures of more than 52°C. Clean the equipment thoroughly between samples. Thoroughly remix the ground sample and store it in an airtight container to avoid contamination. 4.1.4 Rehydrating—Thoroughly blend and rehydrate samples which contain calcium sulfate in forms other than CaSO4·2H2O and natural anhydrite. Place the sample in distilled water and keep it wet for not less than 48 h. Dry the hydrated sample in an oven at 45 6 3°C to constant weight and recrush or grind it in accordance with 4.1.3. 4.1.5 Sample Reduction—Thoroughly mix and reduce large samples as required by quartering or by the use of a riffle to obtain a specimen of approximately 50 g. 4.2 Gypsum (C 22/C 22M)—Gypsum samples will be received in the form of rocks, powder or both. If necessary crush and reduce the entire dried sample in accordance with 4.1.3 and 4.1.5. 4.3 Gypsum Plaster , (C 28). 4.3.1 Gypsum Ready-Mixed Plaster or Gypsum WoodFibered Plaster —Screen the dried sample through a 150-µm (No. 100) sieve6 and discard the residue retained on the sieve. Reweigh the remaining sample and calculate the percentage of the dried sample. Reduce the sample in accordance with 4.1.5. Thoroughly blend and rehydrate the specimen in accordance with 4.1.4. 4.3.2 Gypsum Neat Plaster or Gypsum Gauging Plaster — Reduce the dried sample in accordance with 4.1.5. Thoroughly blend and rehydrate the specimen in accordance with 4.1.4. 4.4 Gypsum Casting and Molding Plaster , (C 59)—Reduce the dried sample in accordance with 4.1.5. Thoroughly blend and rehydrate the specimen in accordance with 4.1.4. 4.5 Gypsum Keene’s Cement , (C 61)—Reduce the dried sample in accordance with 4.1.5. Blend in no more than 1 % molding plaster or K 2SO4 and rehydrate the specimen in accordance with 4.1.4. 4.6 Gypsum Concrete, (C 317)—Screen the dried sample through a 150-µm (No. 100) sieve6 and discard the residue retained on the sieve. Reweigh the remaining sample and calculate the percentage of the dried sample. Reduce the sample in accordance with 4.1.5. Thoroughly blend and rehydrate the specimen in accordance with 4.1.4. 4.7 Gypsum Board —Cut or break the dried sample into small pieces. Using a mortar and pestle, strike the pieces of the sample to loosen the paper face. Remove the pieces of paper by hand as they are separated from the core of the gypsum board. Carefully scrape any remaining powder from the paper. When all the paper has been removed from the pieces of the sample, reduce the sample in accordance with 4.1.5. Thoroughly blend and rehydrate the specimen in accordance with 4.1.4.
Detailed requirements for this sieve are given in Speciﬁcation E 11.
COMPLETE PROCEDURE 5. Apparatus 5.1 Analytical Balance—Capable of weighing the weighing bottles, lids and samples. 5.2 Balance—Capable of weighing not less than 100 g at a precision of 0.001 g. 5.3 Drying Oven—A mechanical convection oven set at 45 6 3°C. 5.4 Desiccator —Capable of being tightly sealed and containing calcium chloride or equivalent desiccant. 5.5 Calcining Oven or Furnace—Capable of achieving and maintaining temperatures to not less than 1000°C. 5.6 Weighing Bottles—Borosilicate glass or ceramic containers with tightly sealable lids. 5.7 Hot Plate—A controllable hot plate capable of heating casseroles to approximately 120°C. 5.8 Porcelain Casseroles—With a capacity of 50 to 100 mL. 5.9 Filtering Funnels. 5.10 Filter Paper —Ashless ﬁlter paper Whatman #42 or equivalent.7 5.11 Porcelain Crucibles. 5.12 Mortar and Pestle. 5.13 Mechanical Jaw Crusher —Capable of crushing gypsum rocks up to 50 mm diameter. 5.14 Mechanical Grinder —Burr mill or equivalent capable of grinding the granular output of the jaw crusher speciﬁed in 5.13. 6. Reagents 6.1 Purity of Reagents—Use reagent grade chemicals in all tests. Unless otherwise indicated, use reagents that conform to the speciﬁcations of the Committee on Analytical Reagents of the American Chemical Society, where such speciﬁcations are available.8 If it is necessary to use other grades ﬁrst ascertain that the reagent is of sufficiently high purity so that its use will not lessen the accuracy of the determination. 6.1.1 Ammonium Chloride (NH4Cl). 6.1.2 Ammonium Hydroxide (sp gr 0.90)—Concentrated ammonium hydroxide (NH 4OH). 6.1.3 Ammonium Nitrate (25 g/L)—Dissolve 25 g of ammonium nitrate (NH 4NO3) in water and dilute to 1 L. 6.1.4 Ammonium Oxalate ((NH4)2C2O4). 6.1.5 Barium Chloride (100 g/L)—Dissolve 100 g of barium chloride (BaCl 2·2H2O) in water and dilute to 1 L. 6.1.6 Calcium Chloride (CaCl2)—Anhydrous Calcium Chloride with a combined water of not more than 5 %. 6.1.7 Hydrochloric Acid (sp gr 1.19)—Concentrated hydrochloric acid (HCl). 6.1.8 Hydrochloric Acid (1 + 4)—Mix 1 volume of HCl (sp gr 1.19) with 4 volumes of water. 7 Whatman No. 42 or an equivalent ﬁlter paper has been found suitable for this purpose. 8 Reagent Chemicals, American Chemical Society Speciﬁcations , American Chemical Society, Washington, DC. For suggestions on the testing of reagents not listed by the American Chemical Society, see Analar Standards for Laboratory Chemicals, BDH Ltd., Poole, Dorset, U.K., and the United States Pharmacopeia and National Formulary, U.S. Pharmacopeial Convention, Inc. (USPC), Rockville, MD.
C 471M 6.1.9 Hydrochloric Acid (1 + 5)—Mix 1 volume of HCl (sp gr 1.19) with 5 volumes of water. 6.1.10 Nitric Acid (sp gr 1.42)—Concentrated nitric acid (HNO3). 6.1.11 Potassium Chromate Solution (100 g/L)—Dissolve 5 g of potassium chromate (K 2 CrO4) in 50 mL of water, mix, add 10 drops of 0.05 N silver nitrate (AgNO 3) solution, allow to stand for 5 min, and ﬁlter. 6.1.12 Potassium Permanganate (5.6339 g/L)—Dissolve 5.6339 g of potassium permanganate (KMnO 4) in water and dilute to 1 L. 6.1.13 Silver Nitrate, Standard Solution (0.05 N)—Prepare and standardize a 0.05 N silver nitrate (AgNO 3) solution. 6.1.14 Sodium Ammonium Phosphate—(NaNH4HPO4). 6.1.15 Sulfuric Acid (sp gr 1.84)—Concentrated sulfuric acid (H2SO4). 6.1.16 Sulfuric Acid (1 + 6)—Carefully mix 1 volume of H2SO4 (sp gr 1.84) with 6 volumes of water. 6.1.17 Nitric Acid (0.1 N)—Mix 1.4 mL of HNO3(sp gr 1.42) with 200 mL of water. 6.1.18 Phenolphthalein Indicator Solution— Dissolve 0.25 g of phenolphthalein in 30 mL of methanol and dilute to 50 mL with water. 6.1.19 Sodium Hydroxide Solution (0.1 N)—Dissolve 1 g of sodium hydroxide (NaOH) in 250 mL of water. 6.1.20 Water —Reagent water shall be in accordance with Speciﬁcation D 1193, type II. Speciﬁcation D 1193 gives the following values for type II grade water. Electrical conductivity, max, µS/cm at 298 K (25-C) Electrical resistivity, min, M V·cm at 298 K (25-C) Total organic carbon (TOC), max, µg/L Sodium, max, µg/L Chlorides max, µg/L Total silica, max, µg/L
1.0 1.0 50.0 5.0 5.0 5.0
7. Free Water 7.1 Signiﬁcance and Use—The free water analysis determines the amount of free water contained in the sample as opposed to chemically combined water, and prepares the sample for further analysis. 7.2 Procedure: 7.2.1 Weigh a sample of the material as received of not less than 50 g to a precision of 0.001 g and spread it out in a thin layer in a suitable vessel. Place in an oven and dry at 45 6 3°C for 2 h, then cool in a desiccator and weigh again. The loss of weight corresponds to the free water. 7.2.2 Retain the sample in a sealed container or in the desiccator for further analysis. 7.3 Calculation and Report —Calculate and report loss in weight as a percentage of the sample as received or of the dried sample as required. 7.4 Precision and Bias—Neither the precision nor the bias for the free water analysis has been determined. 8. Combined Water 8.1 Signiﬁcance and Use—The combined water analysis determines the percent of chemically combined water and is used to calculate the purity of gypsum or the amount of gypsum or gypsum plaster in gypsum products. 8.2 Interferences—Some materials, such as organic and
hydrated compounds that decompose within the same temperature range as gypsum, will cause high results. When the maximum temperature is exceeded, some carbonates undergo decomposition, which will result in high results. 8.3 Procedure: 8.3.1 For each sample, place three weighing bottles with lids in the preheated calcining oven or furnace and heat for 2 h at 215 to 230°C. Place in the desiccator and allow to cool to room temperature. Weigh the bottles and lids to the nearest 0.0001 g and record the tare weights. 8.3.2 Weigh out three specimens of approximately 1 g each of the sample as prepared in Section 4 and dried in Section 7 to a precision of 0.0001 g in the previously tared weighing bottles and record the total weight with lids. 8.3.3 Place the specimens in the calcining oven with the lids placed loosely on each bottle or crucible for 2 h or until constant weight has been obtained. 8.3.4 Place the lids tightly on the weighing bottles, remove from the oven, and place in the desiccator to cool to room temperature. 8.3.5 Weigh each specimen to a precision of 0.0001 g and record the weights. 8.3.6 Retain the residues for carbon dioxide analysis. 8.4 Calculation and Report —Calculate and report the average loss in weight of the three specimens as a percentage of the sample as received or of the dried sample, as required, to the nearest 0.001 g and record the tare weights. 8.5 Precision and Bias—Neither the precision nor the bias for the combined water analysis has been determined. 9. Carbon Dioxide 9.1 Summary of Test Method —The sample is decomposed with HCl and the liberated CO 2 is passed through a series of scrubbers to remove water and sulﬁdes. The CO 2 is absorbed with Ascarite, a special sodium hydroxide absorbent, 9 and the gain in weight of the absorption tube is determined and calculated as percent CO 2. 9.2 Signiﬁcance and Use—The carbon dioxide analysis is useful in estimating carbonates and organic carbon for chemical balance. 9.3 Special Reagents: 9.3.1 Magnesium Perchlorate Desiccant 10—for drying. 9.3.2 Sodium Hydroxide Absorbent 9—a coarse sodium hydroxide coated silica. 9.4 Special Apparatus—The apparatus illustrated in Fig. 1 consists of the following: 9.4.1 Purifying Jar A, Fleming, containing sulfuric acid. 9.4.2 Drying Tube B, U-shaped with side arms and glassstoppers. Side arms are shaped to hold rubber tubing. Contains Anhydrone on left side and Ascarite on right side. 9.4.3 Erlenmeyer Flask C , 250 mL, 24/20 ground-glass joint. 9.4.4 Separatory Funnel D, with ground glass stopper and interchangeable hollow ground-glass joint. A delivery tube 9 Ascarite, manufactured by Arthur H. Thomas has been found satisfactory for this purpose. 10 Anhydrone, manufactured by J. T. Baker Inc. has been found satisfactory for this purpose.
FIG. 1 Apparatus for Carbon Dioxide Analysis
bent at the end extends into the sample ﬂask approximately 15 mm from the bottom and is used to introduce acid into ﬂask. 9.4.5 Condenser E . 9.4.6 Gas-Washing Bottle F , 250 mL, with ﬁtted disk containing distilled water to retain most of the acid volatilized from the alkalimeter. 9.4.7 U-Tube G, containing mossy zinc to remove the last traces of HCl. 9.4.8 Gas Washing Bottle H , 250 mL, with fritted disk, containing concentrated H 2SO 4 and trap I , to remove any SO 3 mist that is carried over. 9.4.9 Absorption Bulb J , containing Anhydrone to remove last traces of water vapor. 9.4.10 CO2 Absorption Bulb, containing Ascarite ﬁlled as follows: On the bottom of the bulb, place a layer of glass wool extending above the bottom outlet and on top of this a layer of Anhydrone approximately 10 mm thick; immediately above this place another layer of glass wool, then add Ascarite to almost ﬁll the bulb. Place a top layer of Anhydrone approximately 10 mm thick on top of the Ascarite and top it off with a covering of glass wool. 9.4.11 U-Guard Tube L, ﬁlled with Anhydrone in left side and Ascarite in right side. 9.4.12 Purifying Jar M , Fleming, containing H 2SO4. 9.5 Procedure: 9.5.1 After drying as described in Section 8 place the residue obtained in the 250 mL Erlenmeyer ﬂask ( C ). Connect the ﬂask to the apparatus as shown in Fig. 1. Purge the system free of carbon dioxide by passing a current of CO 2-free air through the apparatus for 10 to 15 min. 9.5.2 Weigh the absorption bulb to 0.0001 g and attach it to the train. Remove the glass stopper from the separatory funnel, place 50 mL of dilute HCl (1 + 1) in the separatory funnel ( D) and replace the stopper with the interchangeable hollow ground-glass joint through which passes a tube for admitting puriﬁed air. Open the stopcock of the separatory funnel and admit air through the top of the funnel to force the hydrochloric acid into the Erlenmeyer ﬂask ( C ). 9.5.3 Start cold water circulating through the condenser ( E ) and, with CO2-free air passing at a moderate rate through the absorption train, place a small hot plate or gas burner under the sample ﬂask and boil for approximately 2 min. Remove the hot plate and continue the ﬂow of puriﬁed air at approximately three bubbles per second for 10 min to sweep the apparatus free
of CO2. Close the absorption bulb, disconnect it from the train and weigh, opening the stopper momentarily to equalize the pressure. Use a second absorption bulb as counterpoise in all weighings unless a single pan balance is used. 9.6 Calculation—Calculate the percent CO2 to the dried sample as follows: Percent CO 2 5 ~~ A 2 B ! / C 3 100 !~1 2 D !
where: A = mass of absorption bulb + CO2 g, B = mass of absorption bulb before the run, g, C = mass of specimen, g, and D = percent combined water as determined in Section 8 as a decimal. Calculate the percent CO2 to the sample as received as follows: Percent CO 2 5 E ~1 2 F !
where: E = result of Eq 1, and F = percent free water as determined in Section 7 as a decimal. 9.7 Precision and Bias—Neither the precision nor the bias for the carbon dioxide analysis has been determined. 10. Silicon Dioxide and Other Acid Insoluble Matter 10.1 Summary of Test Method —The gypsum and other acid soluble components of the sample are dissolved in dilute hydrochloric acid (HCl). The residue is weighed and calculated as silicon dioxide and other acid insoluble matter. 10.2 Signiﬁcance and Use—The silicon dioxide and other acid insoluble matter analysis determines and is used to report the percentage of one of the inert impurities in gypsum and gypsum products. 10.3 Procedure—Perform in triplicate. 10.3.1 Weigh approximately 1 g of the specimen prepared in Section 4 to the nearest 0.0001 g. 10.3.2 Place the specimen in a porcelain casserole. Add approximately 50 mL of 1 + 5 hydrochloric acid. Evaporate slowly and carefully to apparent dryness on a hot plate. Take not less than 20 min to do the evaporation. Make a blank determination with one casserole in parallel. Cool to room temperature. 10.3.3 Add enough hydrochloric acid (sp gr 1.19) to wet the
C 471M solid residue. Add 20 mL of water, boil and ﬁlter through ﬁlter paper.7 Wash the ﬁlter paper thoroughly using not less than 100 mL of room temperature water to render the precipitate chloride free. The most effective washing technique is to use many small quantities of wash water rather than ﬁll the funnel to the brim two or three times. Test the ﬁltrate for chloride by collecting a small amount and adding a few drops of 0.1 normal silver nitrate (AgNO3) solution. A white precipitate indicates more washing is needed. Discard this test solution. 10.3.4 Place all the ﬁltrate back in the same casserole. Evaporate to dryness and heat to 120°C for 1 h and cool. To the cooled casserole add enough HCl (sp gr 1.19) to wet the solid residue. Add 50 mL of water and boil. 10.3.5 Wash the second contents of the casserole through another ﬁlter 7 paper. Thoroughly wash the residue in the ﬁlter paper until chloride free as in 10.3.3. Retain the ﬁltrate for the iron and aluminum oxide analysis. 10.3.6 Dry sufficient crucibles by placing in a cold muffle furnace during warm up or by placing in a drying oven for 15 to 20 min, then placing in a 900°C muffle furnace. Cool crucibles to room temperature in a desiccator. 10.3.7 Transfer both ﬁlter papers to a tared crucible and char slowly without ﬂaming. Burn off all the carbon and ignite in a muffle furnace at 900°C for 15 min. 10.3.8 Cool the crucibles in a desiccator and weigh to the nearest 0.0001 g. 10.4 Calculation and Report —Calculate the average weight of the three precipitates and report as silicon dioxide (SiO 2) and other insoluble matter to the percentage of sample as received or to the dried sample as required. 10.5 Precision and Bias—Neither the precision nor the bias for the silicon dioxide and other acid insoluble matter has been determined. 11. Iron and Aluminum Oxides 11.1 Signiﬁcance and Use—The iron and aluminum oxides (Fe2O3 + Al2O 3) analysis is used to determine the quantity of these metal oxides in gypsum or gypsum products. 11.2 Procedure—To the ﬁltrate, obtained as described in Section 10, add a few drops of nitric acid (HNO 3), and boil to ensure oxidation of the iron. Add 2 g of ammonium chloride (NH4Cl) previously dissolved in water. Make alkaline with ammonium hydroxide (NH 4OH). Digest hot for a few minutes until the precipitate coagulates. Filter, wash, ignite the precipitate at 1000°C for 30 min or to constant weight in a muffle furnace and weigh as Fe 2O3 + Al2O3. Save the ﬁltrate for the CaO analysis. NOTE 2—The addition of a pinch of ashless ﬁlter paper pulp will aid in the ﬁltration of the precipitate.
11.3 Calculation—Calculate Fe2O3 + Al2O3 to the percentage of sample as received or the dried sample as required. This precipitate may be further treated to separate the two oxides, but this is generally unnecessary. 11.4 Precision and Bias—Neither the precision nor the bias for the iron and aluminum oxides analysis has been determined. 12. Calcium Oxide 12.1 Signiﬁcance and Use—The calcium oxide (CaO)
analysis is used to determine the amount of CaO and calculate the amount of calcium carbonate (CaCO 3) in gypsum and gypsum products. 12.2 Procedure: 12.2.1 To the ﬁltrate obtained as described in Section 11 add 5 g of ammonium oxalate ((NH 4)2C2O4) dissolved in water. Digest hot for 30 min, making sure that the solution is always alkaline with NH 4OH. Filter, wash, and ignite the precipitate at 1000°C for 2 h to constant weight in a platinum crucible in a muffle furnace. 12.2.2 Alternative Method —To the ﬁltrate obtained as described in Section 11, add 5 g of (NH 4)2C2O4 dissolved in water. Digest hot for 30 min, making sure that the solution is always alkaline with NH4OH. Filter and wash, transfer the precipitate to a beaker, and wash the ﬁlter paper with hot H2SO4(1 + 6), catching the washing in the same beaker. Heat gently to complete solution, adding more H 2SO4 if necessary. While still warm, titrate with potassium permanganate (KMnO4) solution (5.6339 g/L) until the pink color persists. 12.3 Calculation—The number of milliliters of KMnO 4 solution used gives directly the percentage of lime in the dried sample. Calculate the CaO to the percentage of sample as received or the dried sample as required. 12.4 Precision and Bias—Neither the precision nor the bias for the calcium oxide analysis has been determined. 13. Magnesium Oxide 13.1 Signiﬁcance and Use —The magnesium oxide (MgO) analysis is used to determine the amount of MgO and calculate the amount of magnesium carbonate MgCO 3 in gypsum and gypsum products. 13.2 Procedure—To the ﬁltrate obtained as described in 12.2.1 or 12.2.2, add enough water to give a total volume of approximately 600 mL. Cool, and add 10 mL of NH 4OH and 5 g of sodium ammonium phosphate (NaNH 4HPO4) dissolved in water. Stir vigorously until a precipitate begins to form. Let stand overnight. Filter, using a Gooch crucible, and wash with NH4NO3 solution. Ignite at 1000°C for 2 h to constant weight in a muffle furnace. 13.3 Calculation—Multiply this weight by 0.36207 to ﬁnd the weight of magnesium oxide (MgO). Calculate the MgO to the percentage of sample as received or to the dried sample as required. 13.4 Precision and Bias—Neither the precision nor the bias for the magnesium oxide analysis has been determined. 14. Sulfur Trioxide 14.1 Summary of Test Method —In this test method, sulfate is precipitated from an acid solution of the gypsum with barium chloride (BaCl2). The precipitate is ﬁltered and weighed as barium sulfate (BaSO 4) and the sulfur trioxide (SO 3) equivalent is calculated. 14.2 Signiﬁcance and Use—The speciﬁcation for gypsum and some gypsum products speciﬁes the amount of calcium sulfate (CaSO4) required, either in the dihydrate (CaSO 4· 2H2O) or hemihydrate (CaSO 4· 1 ⁄ 2H2O) form. This procedure assumes that an insigniﬁcant amount of sulfate other than
C 471M calcium sulfate is present. This test method is used to determine compliance to the gypsum and gypsum product speciﬁcations. It is also commonly used in quality control work. 14.3 Interference—This test method has been developed for natural gypsum and for impurities generally found associated with natural gypsum. Synthetic gypsum will sometimes have an additional number of interfering elements and compounds, and if so, this procedure will not give accurate results. This test method has a number of interferences that theoretically affect the results. Co-precipitation and occlusion are problems if the solution is either too acidic or too basic. Calculations using SO3 analysis are most accurate on samples that are known to be completely hydrated or completely dehydrated. 14.4 Procedure: 14.4.1 Having properly selected and prepared the samples as speciﬁed in Section 4, weigh a representative specimen of approximately 0.5 g, to the nearest 0.0001 g. 14.4.2 Place the weighed sample into a 400-mL beaker. Add 50 mL of HCl (1 + 5). Boil and disperse with the ﬂattened end of a glass rod while stirring until the sample is completely broken down. Add approximately 100 mL boiling water and continue boiling for 15 min, with this step to be extended as required, so the combined boiling time is not less than 1 h. 14.4.3 Using ﬁlter paper7, ﬁlter into a clean 600-mL ﬂask and rinse the 400-mL beaker thoroughly with hot distilled water. Carefully wash the sides of the 400-mL beaker while wiping the insides with a rubber-tipped glass rod making sure all splatters and insoluble are washed into the ﬁlter paper. Dry and burn off the ﬁlter paper leaving the residue to be dried and weighed for insoluble matter, if this test method is not otherwise conducted. 14.4.4 Dilute the ﬁltrate to 400 to 500 mL. Add 1 to 2 drops of 0.1 % methyl red indicator. Prepare a 400 to 500-mL sample of 0.05 to 0.1 NHCl. Add 1 to 2 drops of 0.1 % methyl red indicator. Compare the color of this solution to the color of the ﬁltrate. Dilute the ﬁltrate or add HCl (1 + 5) solution as necessary to match the pH of the 0.05 to 0.1 NHCl solution. 14.4.5 Boil the ﬁltrate solution and add 20 mL of nearboiling 10 % barium chloride solution, preferably with the help of a pipette, drop by drop while stirring. The barium chloride solution should be prepared not less than one day before use. Continue boiling the solution for 10 to 15 min and digest hot for 3 h or until the precipitate settles. 14.4.6 Filter7 and wash with approximately 125 to 150 mL of hot water to render the precipitate chloride free. Test the ﬁltrate for chloride by collecting a small amount and adding a few drops of 0.1 N AgNO3 solution. A white precipitate indicates more washing is needed. Alternately, use ﬁltering crucibles11 for quick ﬁltering if the particular crucibles to be used are tested prior to use by reﬁltering the ﬁltrate from the crucibles with ﬁlter paper, and no more than 2 mg is collected on the ﬁlter paper. 14.4.7 Ignite the precipitate and paper in a tared crucible, and slowly char the paper without inﬂaming. Burn off all the carbon and ignite in a muffle furnace at 800 to 900°C or using bright red heat over a Bunsen burner for 15 to 20 min. Dry the
ﬁltering crucibles by placing in a cold muffle furnace during warm-up or in a drying oven prior to igniting in a muffle furnace at 800 to 900°C for 15 to 20 min. NOTE 3—Thoroughly cleans crucibles before each use and heat in a furnace at 800 to 900°C and cool in a desiccator before taring.
14.4.8 Cool all crucibles in a desiccator and weigh to the nearest 0.0001 g. 14.5 Calculation—Multiply the weight of the precipitate by 0.343 to determine the weight of sulfur trioxide (SO 3). Calculate the SO3 to the percentage of sample as received or to the dried sample as required. 14.6 Precision and Bias—Neither the precision nor the bias for the sulfur trioxide analysis has been determined. 15. Chlorides 15.1 Signiﬁcance and Use—Small amounts of chlorides in gypsum or gypsum products often have a detrimental effect on their use. This procedure is used to measure the amount of chlorides present and report it as sodium chloride. 15.2 Procedure: 15.2.1 Weigh approximately 20.0 g of sample as prepared in Section 4 to 0.001 g and transfer to a 400-mL beaker. Add 150 mL of water, stir, and heat to just below the boiling point. Cover with a watch glass and maintain at just below boiling (not less than 80°C) for 1 h with occasional stirring. Filter with suction on a Buchner funnel ﬁtted with a medium ﬁlter paper. Wash the residue with four 20-mL portions of hot water. 15.2.2 Add 2 drops of phenolphthalein indicator solution to the ﬁltrate. If the ﬁltrate fails to turn pink, add 0.1 NNaOH solution dropwise with stirring until a faint pink color develops. Add 0.1 NHNO3 dropwise until the pink color just disappears. 15.2.3 If the chloride content is very low, transfer the entire ﬁltrate quantitatively to a 400-mL beaker and proceed as described in 15.2.4. If larger amounts of chloride are expected, transfer the ﬁltrate quantitatively to a 250-mL volumetric ﬂask, cool to room temperature, and dilute to 250 mL. Take a suitable aliquot, transfer to a 400-mL beaker, and dilute to a volume of 100 to 250 mL. 15.2.4 Place the beaker containing the sample on a white surface, add 0.5 mL (10 drops) of K 2CrO4 solution and titrate with AgNO3 solution using a micro buret having a 10-mL capacity and graduated in divisions of 0.02 mL. Titrate until a faint but deﬁnite orange color is visible. 15.2.5 Perform a blank titration using the same volume of water as the sample volume and the same amount of K 2CrO4 solution. Titrate to the same color as obtained with the sample. 15.3 Calculation—Subtract the volume of AgNO 3 solution used for the blank titration from the volume used for the sample to give the net titration. A 1-mL net titration is equivalent to 0.002923 g of sodium chloride (NaCl). Calculate the NaCl as a percentage of the sample as received or the dried sample as required. 15.4 Precision and Bias—Neither the precision nor the bias for the chloride analysis has been determined. 16. Report
Gooch or Coors ﬁltering crucibles have been found suitable for this purpose.
16.1 Report the results obtained in the analysis as follows:
C 471M Free water Combined water Carbon dioxide (CO2) Silicon dioxide (SiO 2) and insoluble matter Iron and aluminum oxides (Fe 2O3 + Al2O3) Lime (CaO) Magnesium oxide (MgO) Sulfur trioxide (SO3) Sodium chloride (NaCl) Total
Percent ... ... ... ... ... ... ...
18.2 Ammonium Hydroxide Wash Solution— Dilute 100 mL of concentrated ammonium hydroxide (NH 4OH, sp gr 0.90) to 1 L with water. 18.3 Filter Aid —Diatomaceous silica, analytical grade. 18.4 Phenolphthalein Indicator Solution.
19.1 Weigh rapidly approximately 4 g of the well-mixed sample and transfer to a 600-mL beaker. Make all weighings to 0.001 g, except weigh the crucibles and their contents to 0.0001 g. 19.2 Without delay, weigh approximately 1 g of the wellmixed sample in a tared weighing bottle having a ground-glass stopper. Dry the sample and weighing bottle to constant weight at 45°C. Stopper weighing bottles immediately upon removal from the oven in order to prevent absorption of moisture from the air upon cooling. 19.3 If the percentage by weight of combined water held by the calcium sulfate is required, heat the sample and weighing bottle to constant weight at 220°C. 19.4 To the contents of the 600-mL beaker (19.1), add 350 mL of the ammonium acetate solution, and stir the mixture thoroughly to loosen all of the solid matter from the bottom of the beaker. Add 0.2000 g of redried diatomaceous silica to the mixture. Heat the beaker and contents to 70°C on a steam or hot water bath, and maintain at that temperature for 30 min, while stirring frequently. During heating, keep the solvent ammoniacal by additions of NH 4OH and phenolphthalein, if indicated. Meanwhile, heat a supply of the ammonium acetate solution to 70°C, keeping it also distinctly ammoniacal. Filter the mixture, with suction, through a tared Gooch crucible, stirring frequently during ﬁltration to keep the diatomaceous earth suspended in the liquid. Wash the Gooch crucible containing the residue with ﬁve 10-mL portions of the warm acetate solution, draining thoroughly after each washing. Wash in the same manner with eight 10-mL portions of the NH 4OH wash solution. Take care to wash the upper walls of the Gooch crucible. Drain the crucible dry with suction, place in an oven at 70°C, and dry to constant weight (Note 7). Allow the crucible to cool in a desiccator before weighing.
NOTE 4—Since it is frequently advisable to recalculate the results obtained in the chemical analysis in order that they may be more enlightening, the following is submitted for consideration: (1) Multiply the percentage of combined water by 4.778 to obtain purity or percentage gypsum. To calculate the percentage of CaSO4· 1 ⁄ 2H2O in plasters, multiply the percentage of gypsum by 0.8430. (2) Multiply the percentage of combined water by 2.222 to obtain the amount of SO3 combined as gypsum. (3) Subtract the result obtained in (2) from the total SO3 found by analysis to obtain the excess SO3. (4) Multiply the excess SO3 by 1.700 to obtain the percentage anhydrite, CaSO4. (5) Multiply the percentage of gypsum found in (1) by 0.3257 to obtain the percentage of CaO combined as gypsum. (6 ) Multiply the percentage of anhydrite found in (4) by 0.4119 to obtain the percentage of CaO combined as anhydrite. (7 ) Add (5) and (6 ) together. Then subtract this result from the total CaO percentage found by analysis. (8 ) Multiply the excess CaO percentage by 1.785 to obtain the percentage of calcium carbonate. (9) Multiply the percentage of MgO by 2.091 to obtain the percentage of magnesium carbonate. NOTE 5—Having made the calculations in Note 4, the results may be reported as follows: Gypsum (CaSO4·2H2O) Anhydrite (CaSO4 natural and manufactured) (Note 4) Silicon dioxide and insoluble (SiO 2 + Ins.) Iron and aluminum oxide (R 2O3) Calcium carbonate (CaCO3) Magnesium carbonate (MgCO3) Sodium chloride (NaCl) Total
Percent ... ... ... ... ... ... ... 100.006
NOTE 6—The presence of the different forms of CaSO4 may be determined by a microscopic examination. A paper titled “Gypsum Analysis with the Polarizing Microscope” containing suggested methods can be found in ASTM STP 861.12
ALTERNATIVE PROCEDURE FOR ANALYSIS FOR CALCIUM SULFATE BY THE AMMONIUM ACETATE METHOD13
19. Procedure Using Gooch Crucible
NOTE 7—Avoid overheating in all oven drying of ammonium acetate residues; that is, place crucibles well away from the heating elements. This is of particular importance for samples high in impurities, as these impurities often have water of hydration that is lost on local overheating.
17. Signiﬁcance and Use
20. Procedure Using Tared Filter Papers
17.1 This test method covers the determination of calcium sulfate in gypsum and gypsum products by extraction with ammonium acetate solution.
NOTE 8—This procedure is suggested where several samples are to be analyzed at once. It has been found that gravity ﬁltration on six samples will proceed as rapidly as it is possible to handle the samples.
18. Reagents and Materials 18.1 Ammonium Acetate Solution—Dissolve 454 g of ammonium acetate in 2 L of water. Add sufficient NH 4OH to make the solution distinctly ammoniacal, using phenolphthalein as the indicator. 12 Green, George W., “Gypsum Analysis with the Polarizing Microscope,” The Chemistry and Technology of Gypsum, ASTM STP 861 , ASTM, 1984, pp. 22–47. 13 This procedure was developed by L. S. Wells and W. F. Clarke, National Bureau of Standards, and modiﬁed by B. E. Kester, United States Gypsum Co.
20.1 Dry a quarter-folded, 110-mm quantitative ﬁlter paper 7 overnight at 70°C in a wideform, glass-stoppered, 30 by 60-mm weighing bottle. After drying, cool the weighing bottle and paper in a desiccator, and weigh. 20.2 Treat the sample exactly as described in 19.1, 19.2, and 19.4 prior to the ﬁltration. Filter the mixture by gravity through a 70-mm glass funnel, stirring frequently during ﬁltration to keep the diatomaceous silica suspended in the liquid. Wash the ﬁlter paper and residue with ﬁve 10-mL portions of warm acetate solution, draining thoroughly after each washing. Wash
C 471M in the same manner with eight 10-mL portions of the NH 4OH wash solution. After ﬁnal draining, replace the paper and residue in the weighing bottle, and dry at 70°C to constant weight. Cool the weighing bottle, paper, and residue in a freshly prepared desiccator before weighing; this is essential, due to the hygroscopic character of paper. 21. Calculation 21.1 Calculate the percentage of loss in weight at 45°C (free water) as follows: Loss in weight at 45°C , % 5 @~ A 2 B ! / C # 3 100
where: A = original weight of sample and weighing bottle, B = weight of sample and weighing bottle dried to constant weight at 45°C, and C = original weight of sample. Calculate the weight of the 4-g sample (19.1), corrected for loss on heating to constant weight at 45°C. 21.2 Calculate the percentage of combined water as follows: Combined water, % 5 @~ B 2 D ! / ~ B 2 E !# 3 100
where: B = weight of sample and weighing bottle dried to constant weight at 45°C, D = weight of sample and weighing bottle dried to constant weight at 220°C, and E = weight of weighing bottle. 21.3 Calculate the percentage of CaSO4· nH2O on the basis of the sample dried to constant weight at 45°C as follows: CaSO 4 · nH 2O, % 5 @ F 2 ~ G 2 H ! / F # 3 100
where: F = weight of sample, corrected for loss on heating to constant weight at 45°C, G = weight of dried crucible and contents (19.4) or weight of weighing bottle and contents (20.2), and H = weight of crucible plus diatomaceous silica used as ﬁlter aid (19.4), or weight of weighing bottle, diatomaceous silica used as a ﬁlter aid and the weight of ﬁlter paper (20.2). 22. Precision and Bias 22.1 Neither the precision nor the bias for the analysis of calcium sulfate by the ammonium acetate method has been determined. ALTERNATIVE PROCEDURE FOR ANALYSIS FOR SODIUM CHLORIDE BY THE COULOMETRIC METHOD14 23. Signiﬁcance and Use 23.1 This test method covers the determination of sodium chloride in gypsum and gypsum products by the coulometric method. 24. Interferences 24.1 The presence of sulﬁde, sulfhydryl, or other silver 14
This procedure was developed by Westroc Industries Limited.
reactive substances will lead to high results. Such interfering substances are removed by alkaline oxidation with hydrogen peroxide. 25. Apparatus 25.1 Chloride Meter : 25.1.1 The instrument shall be equipped to measure the concentration of dissolved chloride in aqueous solutions by the coulometric method. 15 25.1.2 The instrument shall be capable of measuring chloride concentrations in the range from 10 to 260 mg/L with a repeatability of 6 1 mg/L. 26. Reagents 26.1 Acid Buffer Solution—Dissolve 100 mL of 99.5 % acetic acid (HC 2H3O2) and 5.5 mL of concentrated nitric acid (sp gr 1.42) in approximately 200 mL of water and dilute to 500 mL. 26.2 Diluted Standard Solution (100 mg Cl/L)—Dilute 5.00 mL of stock standard solution to 500 mL. 26.3 Gelatin Solution—Add 2.5 g of gelatin and 0.5 g of thymol blue to 250 mL of water and dissolve by stirring continuously while bringing to a boil. With the solution just boiling, continue stirring until all the thymol blue is dissolved. Add 0.5 g of thymol, cool, and dilute the solution to 500 mL. NOTE 9—The gelatin solution holds the precipitated silver chloride (AgCl) in suspension and also indicates the presence of the acid buffer. The solution will keep for 3 months at room temperature or longer if refrigerated. Warm the refrigerated solution to room temperature before use.
26.4 Stock Standard Solution (10 g Cl/L)—Dissolve 8.240 g of dried sodium chloride (NaCl) in water and dilute to 500 mL. 27. Procedure 27.1 Weigh 20.0 g of the well-mixed sample and transfer to a 150-mL beaker. 27.2 Add 50 mL of water, boil, allow the solid material to settle, and ﬁlter off the solution. Add an additional 50 mL of water to the solids, boil, and pour the contents of the beaker into the ﬁlter. Wash the residue with 100 mL of hot water, adding the washing to the ﬁltrate. Cool and dilute with water to 250 mL. 27.3 Switch on the chloride meter and allow a period of 25 min before use. Set the counter to zero. 27.4 Place a magnetic stirring bar in the test beaker, add 10 mL of diluted standard solution, 3 mL of acid buffer solution, and 5 drops of gelatin solution. Place the test beaker on the platform and lower the electrodes into the solution. Press the “start” button until the pilot light is extinguished. The counter will begin to register after a few seconds. Do not remove the electrodes from the sample until the pilot light comes on. Read the chloride content from the counter. If a reading of 100 6 1
The EEL Chloride Meter, available from Fisher Laboratory Supplies Co., has been found satisfactory. Other instruments available for the coulometric determination of chloride are the Aminco Chloride Titrator, available from American Instrument Co. Ltd.; the Buchler Chloridometer, available from Buchler Instruments Division of Nuclear Chicago Corp.; and the Fiske/Marius Chlor-O-Counter available from Johns Scientiﬁc.
C 471M mg Cl/L is not obtained, refer to the manufacturer’s instruction manual. Reset the counter to zero. 27.5 Repeat the procedure used in 27.4, using 10 mL of the sample solution instead of the diluted standard solution. Read the result as milligrams of chlorine per litre. When all tests are completed, lower the electrodes into reagent water. 28. Calculation 28.1 Calculate the amount of NaCl as a percentage of the sample as received or dried sample as follows: NaCl, % 5 0.00206 3 A
where: A = chloride meter reading, mg Cl/L. 29. Precision and Bias 29.1 Neither the precision nor the bias for the sodium chloride analysis by the coulometric method has been determined. DETERMINATION OF SAND IN SET PLASTER 30. Summary of Test Method 30.1 This test method for the determination of the sand content of set gypsum plaster requires for accurate results the following determinations: 30.1.1 Determination of the percentage of insoluble matter in the sand used with the plaster, 30.1.2 Determination of the percentage of insoluble matter in the gypsum neat plaster, and 30.1.3 Determination of the percentage of insoluble matter in the sanded calcined plaster. NOTE 10—If samples of the original gypsum neat plaster and the sand are not available, an approximation of the insoluble matter may be obtained by the use of this method on plaster and sand from the same sources as those from which the plaster to be analyzed was originally prepared.
31. Signiﬁcance and Use 31.1 This test method is used for determining the sand content of samples of aggregated plaster taken from job sites to determine compliance with Speciﬁcation C 842. 32. Reagents 32.1 Ammonium Acetate (250 g/L)—Dissolve 250 g of ammonium acetate (NH 4C2H3O2) in water and dilute to 1 L. 32.2 Ammonium Hydroxide (1 + 59)—Mix 1 volume of concentrated ammonium hydroxide (NH 4OH) (sp gr 0.90) with 59 volumes of water. 33. Sampling 33.1 Where plaster to be tested is part of a two-coat or three-coat plastering operation, take the sample for analysis from that portion of the entire plaster sheet that comprises the single coat being tested. Separate succeeding coats of plaster by use of a stiff putty knife or similar implement. Not less than 500 g shall be taken as a sample, the sample preferably being obtained from different sections of the wall or ceiling under examination.
34. Procedure 34.1 In a clean porcelain mortar, grind the set plaster sample to the size of the largest sand particles present, or smaller, so that approximately 100 % of the sample will pass a 2.36-mm (No. 8) sieve. Fine grinding makes solution of the gypsum faster. Place approximately 200 g of the ground sample in a porcelain casserole or evaporating dish, and calcine on a sand bath. Stir the sample continuously with a thermometer during the heating, and adjust the rate of heating so that 20 to 30 min will be required to raise the temperature of the sample to 160 6 5°C. Cool the sample to room temperature in a desiccator. 34.2 After cooling, weigh accurately 20 6 0.05 g of the calcined sample into a 600-mL beaker. Add 300 to 350 mL of NH4C2H3O2 solution. If acidic to litmus paper, add a few millilitres of NH 4OH (1 + 59) to the stock NH 4C2H3O2 solution to render it slightly alkaline prior to the addition to the test sample. 34.3 Warm the suspension to a temperature of 70 6 5°C and stir continuously for 20 to 30 min. Filter the warm suspension with the aid of suction through a small Büchner funnel or Gooch crucible in which ﬁlter paper has previously been placed. Reﬁlter the ﬁrst 100 mL of the ﬁltrate. Wash the sand remaining in the beaker onto the ﬁlter with an additional 100 mL of warm ammonium acetate solution. Wash the beaker and residue with 200 to 300 mL of water, dry the funnel and sand at 100°C to constant weight. The weight of the residue is the weight of insoluble matter. 34.4 Insoluble Matter in Sand —Determine the weight of insoluble matter in sand as described in 34.1-34.3, except that no grinding of the sample is necessary. 34.5 Insoluble Matter in Gypsum Neat Plaster —Determine the weight of insoluble matter in the gypsum neat plaster as described in 34.1-34.3, except that only a 5-g sample is required and no grinding of the sample is necessary. 35. Calculation 35.1 Insoluble Matter in Plaster —Multiply by 5 the weight of the insoluble matter obtained as described in 34.3 to obtain the percentage of insoluble matter in sanded plaster. 35.2 Insoluble Matter in Sand —Multiply by 5 the weight of the insoluble matter in sand obtained as described in 34.4 to obtain the percentage of insoluble matter in sand. 35.3 Insoluble Matter in Gypsum Neat Plaster —Multiply by 20 the weight of the insoluble matter in gypsum neat plaster obtained as described in 34.5 to obtain the percentage of insoluble matter in gypsum neat plaster. 35.4 Calculate the percentage of sand in the sanded plaster as follows: X 5 @~ C 2 B ! / ~ A 2 B !# 3 100
where: X = % of sand in sanded plaster, A = % of insoluble matter in the sand, B = % of insoluble matter in the gypsum neat plaster, and C = % of insoluble matter in the sanded plaster. 35.5 To express the results as a ratio of the parts of sand per part of plaster by weight, use the following equation:
C 471M Ratio of sand to plaster 5 X / ~100 2 X !
NOTE 11—The results obtained by the above procedure indicate the amount of sand originally mixed with the gypsum neat plaster before it had been gaged with water or set.
36. Precision and Bias 36.1 Neither the precision nor the bias for the analysis of sand in set plaster has been determined. WOOD-FIBER CONTENT IN WOOD-FIBER GYPSUM PLASTER 37. Signiﬁcance and Use 37.1 This test method is used to determine the weight of wood ﬁber in wood-ﬁbered plaster. 38. Procedure 38.1 Place a 100-g sample of wood-ﬁber plaster, prepared as described in Section 4 on a 600-µm (No. 30) sieve 6 nested over a 150-µm (No. 100) sieve. 6 Wash the plaster on the 600-µm sieve with a stream of cold water, removing the 600-µm sieve when the ﬁber on it is practically or entirely free of plaster. Next, wash the material on the 150-µm sieve until the bulk of the plaster has been washed through the sieve and the residue is mainly ﬁber. Transfer the material retained on the 150-µm sieve to a 300-mL, vitreous enamel, lipped pan, adding the charge on the 600-µm sieve if the ﬁber contains any adhering particles of plaster. Elutriate the material in the pan (purify by washing and straining, effecting as clean a separation of ﬁber from plaster as is practical), catching the elutriated ﬁbers on a 150-µm sieve. To avoid loss of the ﬁne particles of ﬁber, make the transfer from the pan to the 150-µm sieve by several stages of washing, stirring the charge, and quickly pouring upon the sieve the ﬁber ﬂotations, repeating the elutriation procedure several times. Examine the ﬁber collected on the 150-µm sieve and repeat the elutriation if necessary. 38.2 Dry the sieves (or sieve) and the residue contained thereon overnight in an oven maintained at a temperature of 45°C. Carefully invert the sieves, or sieve, over a piece of white paper, and transfer the residual material to the paper by brushing the bottom of the inverted sieve. Examine the transferred material visually, noting whether the separation of ﬁbers from plaster has been complete. Then transfer the material to a weighed platinum crucible and dry to constant weight at a temperature of 45°C. If the previous visual examination of the charge on the white paper showed that the ﬁber was practically free of particles of plaster, report as the percentage of ﬁber the weight of the ﬁber dried at 45°C, divided by 100. If, on the other hand, the visual examination revealed the presence of an appreciable quantity of plaster associated with the ﬁber, carefully ignite the contents of the crucible to constant weight. In this case, report as the percentage of ﬁber the loss on ignition, divided by 100. 39. Precision and Bias 39.1 Neither the precision nor the bias for the analysis of wood-ﬁber content in wood-ﬁber gypsum plaster has been determined.
OPTIONAL PROCEDURE FOR ANALYSIS FOR SODIUM BY THE ATOMIC ABSORPTION METHOD 40. Signiﬁcance and Use 40.1 This test method covers the determination of sodium in gypsum and gypsum products by the atomic absorption method. 41. Interferences 41.1 Sodium is partially ionized in the air-acetylene ﬂame. The effects of ionization will be signiﬁcantly overcome by the addition of 1 to 2 g/L of another alkali to blanks, standards, and samples. Alternatively, use the air-hydrogen ﬂame, as it produces less ionization and less visible emission than the air-acetylene ﬂame. 42. Apparatus 42.1 Atomic Absorption Spectrophotometer : 42.1.1 The instrument shall be equipped to measure the concentration of dissolved sodium in aqueous solutions using either the air-acetylene or air-hydrogen ﬂame. 42.1.2 The instrument shall be capable of measuring sodium concentrations within the optimum analytical range of 0.1 to 0.5 absorbance units while providing a coefficient of variation of approximately 0.5 to 2 %. 43. Reagents 43.1 Solvent —Use deionized water to prepare all solutions. If an alkali is to be included for the purpose of suppressing sodium ionization, it is most convenient to add it to the solvent at the start. In this way a constant concentration of alkali in blank, standards, and sample solution is ensured. 43.2 Stock Standard Solution (1.000 g Na/L)—Dissolve 2.5418 g of dried sodium chloride (NaCl) in water and dilute to 1 L with water. 43.3 Dilute Standard Solutions—Prepare dilute standard solutions bracketing the absorbance range of the dilute sample solution, using the stock standard solution. (Solutions having a concentration less than approximately 0.500 g/L are unstable for periods of more than one day.) 44. Procedure 44.1 Take 18 g of the well-mixed sample and transfer to a 150-mL beaker. 44.2 Add 50 mL of water, boil, allow the solids to settle, and decant the supernatant liquid into a ﬁlter. Add an additional 50 mL of water to the solids, boil, and pour the contents of the beaker into the ﬁlter. Wash the residue with 100 mL of hot water, adding the washing to the ﬁltrate. Cool the ﬁltrate to room temperature and dilute to 500 mL in a volumetric ﬂask to make the stock sample solution. Take 10 mL of the solution and make up to 500 mL in a second volumetric ﬂask, to make the dilute sample solution. 44.3 Determine the absorbance readings on the dilute standard solutions and the solvent blank at a wavelength of 589.0 to 589.6 nm, following the manufacturer’s instruction manual. Subtract the absorbance value for the blank from the absorbance values for the dilute standard solutions and prepare a curve relating sodium concentration in milligrams per litre to absorbance values.
C 471M NOTE 12—If the absorbance of the dilute sample solution is known to lie within the linear range, that is, the sodium concentration is below approximately 1 mg/L only one standard and the solvent blank are needed to prepare the curve.
44.4 Determine absorbance readings on the dilute sample solution using the same technique, followed with the dilute standard solutions. The concentration of sodium in the dilute sample solution in milligrams per litre is then found by consulting the standard curve. 45. Calculation 45.1 Calculate the amount of NaCl as a percentage of the sample received or the dried sample as required as follows: Sodium calculated as % NaCl 5 A 3 6.3553/ S
where: A = concentration of dilute sample solution, mg/L, and S = weight of sample, g. 46. Precision and Bias 46.1 Neither the precision nor the bias for the analysis of sodium by the atomic absorption method has been determined. OPTIONAL PROCEDURE FOR ANALYSIS FOR SODIUM BY FLAME PHOTOMETRY 47. Signiﬁcance and Use 47.1 This test method covers the determination of sodium in gypsum and gypsum products by ﬂame photometry. This test method is based on Methods D 1428. 48. Interferences 48.1 Radiation interferences caused by elements other than that being determined are the greatest contributor to error in ﬂame photometry. Some effects are positive and others negative. Of the elements encountered in this analysis, the greatest effect is that of one alkali metal on another. The foreignelement effects cannot be entirely compensated for without employing calibration standards closely duplicating the composition of the sample. However, the effects are minimized by operating at the lowest practical sodium concentration range or by removal of the interfering elements. For example, aluminum has a depressing effect on alkali-metal emission, which is of serious consequence. Remove aluminum from the extraction liquid prior to ﬂame photometry if its concentration has been found, by preliminary tests, to exceed that of the sodium. 48.2 Self-absorption causes the curve of intensity versus concentration to decrease its slope at higher concentrations, tending to reduce accuracy. Bracketing the unknown by known standard solutions tends to minimize this interference. 49. Apparatus and Materials 49.1 Flame Photometer —The instrument shall consist of an atomizer and burner; suitable pressure-regulating devices and gages for fuel and air or oxygen; an optical system, consisting of suitable light-dispensing or ﬁltering devices capable of preventing excessive interference from light of wavelengths other than that being measured; and a photosensitive indicating device.
49.2 Supply of Fuel and Air or Oxygen — The supplies of fuel and air or oxygen shall be maintained at pressures somewhat higher than the controlled operating pressure of the instrument. 50. Reagents 50.1 Prepare the following stock solutions from reagents that have been dried to constant weight at 105°C. Store the stock solutions in polyethylene or equally alkali-metal-free containers. 50.2 Sodium Chloride Solution (2.5418 g/L)—Dissolve 2.5418 g of sodium chloride (NaCl) in water and dilute to 1 L with water. This stock standard solution contains 1.000 g/L of sodium ion. 50.3 Dilute Standard Solutions—Prepare dilute standard solutions from stock standard solution, bracketing the expected sodium concentration range of the diluted sample extraction liquid. For example, if the expected range of the sample extraction liquid is between 0 and 0.010 g/L, prepare eleven equally spaced standards in tenths of the maximum. 51. Calibration of Instrument 51.1 Select the proper photocell; the blue-sensitive phototube having a range from 320 to 620 nm is required for sodium determination. Open the slit width to approximately one fourth of the maximum opening, set the instrument to the maximum sensitivity range, and balance the meter to obtain electrical equilibrium. 51.2 Feed fuel and air or oxygen to the burner and ignite the emitted mixture. Adjust fuel and air or oxygen pressures and follow the procedures for warm-up time prescribed by the instrument manufacturer. Set the scale-reading dial at approximately 95 % of full scale, introduce a solution containing the maximum amount of sodium in the range to be covered, and allow the emitted light to strike the photocell. 51.3 Select the proper ﬁlter, if a ﬁlter-type instrument is used. For instruments employing spectral dispersing devices, turn the wavelength dial back and forth slowly and carefully in the vicinity of 589 nm until the galvanometer reaches a maximum deﬂection. This wavelength setting produces maximum sensitivity. Do not disturb the wavelength dial during the test. 51.4 Continue to atomize the maximum standard of the range to be covered, and set the scale-reading of the dial at exactly full scale (100 or 1000) (Note 13). Adjust the gain so as to balance the galvanometer needle. NOTE 13—For instruments equipped with a variable slit, carry out the procedure described above with the slit width between fully closed and one fourth open for the preliminary test. In determining the proper slit width for optimum instrument performance, consideration must be given to the fact that the intensity of the emission line is approximately proportional to the slit width, whereas continuous background intensity increases as the square of the slit width. A decrease in slit width results in decreased illumination of the phototube for a given concentration and is compensated for by increasing the gain of the instrument. The most favorable operating conditions are obtained with the smallest slit width that does not result in instability of the galvanometer needle when it is set to give full-scale reading with the maximum standard in the range to be covered. When altering the slit width, determine the background by atomizing a zero standard, and check for sensitivity setting and instrument
C 471M stability with the maximum standard in the range to be covered. Lower ranges require wider slit widths. Determine and record the optimum slit width for each range and element to be covered. Use these values in all subsequent tests.
51.5 Determine the emission intensity of all standards. 51.6 Plot emission intensity (scale reading) versus concentration on linear graph paper. For the lower ranges, the curve thus prepared approximates a straight line but sometimes will not intersect zero because of background intensity. At higher ranges, the curves show a decrease in slope with increasing concentration. Record on graphs all data in regard to slit width, fuel pressure, and air or oxygen pressure.
52.4 Turn the instrument on and feed fuel and air or oxygen to the burner. Ignite the gas mixture. For instruments with an adjustment slit, set the width to the value determined as outlined in Note 13. 52.5 Place the scale-reading dial at maximum. Atomize the sample and allow its emitted light to strike the photocell. Set the wavelength to 589 nm as described and adjust the gain to balance the galvanometer. Determine the emission intensity of the sample. 52.6 Refer to the standard curve prepared above and read off the concentration of sodium ion in the dilute sample solution in milligrams per litre.
52. Procedure 52.1 Weigh 25 g of the well-mixed sample and transfer to a 150-mL beaker. 52.2 Add 50 mL of water, boil, allow the solid material to settle, and decant the supernatant liquid into a ﬁlter. Add an additional 50 mL of water to the solids, boil and pour the contents of the beaker into the ﬁlter. Wash the residue with 75 mL of hot water, adding the washing to the ﬁltrate. Cool and dilute with water to 200 mL in a volumetric ﬂask to make the stock sample solution. 52.3 Take 5 mL of the stock sample solution and make up to 100 mL in a volumetric ﬂask to make the dilute sample solution. NOTE 14—If the concentration of sodium in the sample is found to be greater than the maximum standard, further dilute sample solution with water to bring the concentration within the range. If the concentration of sodium in the sample is less than one tenth of the value of the maximum standard, prepare a new dilute sample solution from the stock sample solution to bring the concentration within the range.
53. Calculation 53.1 Calculate the amount of NaCl as follows: Sodium, calculated as NaCl, % 5 A 3 0.04067
where: A = concentration of sodium, mg/L read off the standard curve. 54. Precision and Bias 54.1 Neither the precision nor bias of the analysis for sodium by ﬂame photometry has been determined. 55. Keywords 55.1 ammonium acetate method; atomic absorption; chemical analysis; coulometric method; ﬂame photometry; gypsum; gypsum concrete; gypsum board; gypsum products; plaster; sand in set plaster; wood-ﬁber plaster
SUMMARY OF CHANGES This section identiﬁes the location of changes to these test methods that have been incorporated since the last issue. Committee C-11 has highlighted those changes that affect the technical interpretation or use of these test methods. (1) Added paragraph 1.3. (2) Revised paragraph 5.6. (3) Revised paragraph 6.1. (4) Revised paragraph 8.2. (5) Revised paragraph 10.3.2. (6) Revised paragraph 14.3. (7) Revised paragraph 14.4.3. (8) Revised paragraph 14.4.6. (9) Revised paragraph 15.1. (10) Revised paragraph 17.1.
(11) (12) (13) (14) (15) (16) (17) (18) (19) (20) (21) (22) (23) (24)
Revised Revised Revised Revised Revised Revised Revised Revised Revised Revised Revised Revised Revised Revised
paragraph 19.3. paragraph 23.1. paragraph 24.1. paragraph 27.4. paragraph 34.2. paragraph 35.5. paragraph 38.1. paragraph 38.2. paragraph 40.1. paragraph 41.1. paragraph 47.1. paragraph 48.1. paragraph 51.3. paragraph 51.6.
ASTM International takes no position respecting the validity of any patent rights asserted in connection with any item mentioned in this standard. Users of this standard are expressly advised that determination of the validity of any such patent rights, and the risk of infringement of such rights, are entirely their own responsibility. This standard is subject to revision at any time by the responsible technical committee and must be reviewed every ﬁve years and if not revised, either reapproved or withdrawn. Your comments are invited either for revision of this standard or for additional standards and should be addressed to ASTM International Headquarters. Your comments will receive careful consideration at a meeting of the responsible technical committee, which you may attend. If you feel that your comments have not received a fair hearing you should make your views known to the ASTM Committee on Standards, at the address shown below.
C 471M This standard is copyrighted by ASTM International, 100 Barr Harbor Drive, PO Box C700, West Conshohocken, PA 19428-2959, United States. Individual reprints (single or multiple copies) of this standard may be obtained by contacting ASTM at the above address or at 610-832-9585 (phone), 610-832-9555 (fax), or [email protected]
(e-mail); or through the ASTM website (www.astm.org).